Upload
others
View
6
Download
0
Embed Size (px)
Citation preview
PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
Cleaving plane-dependent electronic structures of transition metal diarsenides
Gyanendra Dhakal,1 M. Mofazzel Hosen,1 Wei-Chi Chiu,2 Bahadur Singh,3 Cheng-Yi Huang,2 Klauss Dimitri,1
Baokai Wang,2 Firoza Kabir,1 Christopher Sims,1 Sabin Regmi ,1 William Neff,1 Jonathan Denlinger,4 Hsin Lin,5
Dariusz Kaczorowski ,6 Arun Bansil,2 and Madhab Neupane 1,*
1Department of Physics, University of Central Florida, Orlando, Florida 32816, USA2Department of Physics, Northeastern University, Boston, Massachusetts 02115, USA
3Department of Condensed Matter Physics and Materials Science, Tata Institute of Fundamental Research, Mumbai 400005, India4Advanced Light Source, Lawrence Berkeley National Laboratory, Berkeley, California 94720, USA.
5Institute of Physics, Academia Sinica, Taipei 11529, Taiwan6Institute of Low Temperature and Structure Research, Polish Academy of Sciences, Okolna 2, 50-422 Wroclaw, Poland
(Received 16 January 2020; accepted 21 April 2021; published 2 June 2021)
Topological Dirac and Weyl semimetals are currently attracting intense interest due to their exotic physicalproperties. Transition metal diarsenides such as MoAs2 and WAs2 have been reported to harbor very highmagnetoresistance suggesting the possible existence of a topological quantum state, although this conclusionremains dubious. Here, using systematic angle-resolved photoemission spectroscopy (ARPES) measurementsand parallel first-principles calculations, we discuss the electronic structures of TAs2 (T = Mo, W). Two differentcleavage planes of MoAs2 are found to harbor distinctly different surface states. Our experiments show thepresence of Dirac-like dispersions on the (001) plane, which our first-principles calculations ascribe to trivialsurface states. Our in-depth study also finds WAs2 to possess a trivial electronic structure. Our study emphasizesthe importance of identifying the cleavage plane in low-symmetry systems and indicates that topologicalsemimetallic states are not the key for generating high magnetoresistance in MoAs2 and WAs2.
DOI: 10.1103/PhysRevResearch.3.023170
I. INTRODUCTION
Experimental discovery of a 3D topological insulator stateis widely acknowledged as a major milestone in condensedmatter and materials physics [1–5]. This discovery has spurredintense research interest in other classes of topological mate-rials, and exotic states such as the Dirac semimetal [6–12],Weyl semimetal [13–19], and nodal-line semimetal [20–23]have been theoretically proposed and experimentally realized.In Dirac semimetals, linearly-dispersing bands cross at lowenergies and behave like Dirac fermions. Since inversion andtime-reversal symmetries protect the Dirac states, their re-alization requires the material to be centro-symmetric andnonmagnetic [24,25]. Breaking either the inversion or thetime-reversal symmetry drives a Dirac semimetal into a Weylsemimetal. Weyl fermions evolve as low-energy excitations attopologically protected crossing points (Weyl nodes) betweenthe electron and hole bands. Weyl nodes act as monopoles orantimonopoles of Berry curvature depending on their chirality.Pairs of nodes of opposite chiralities are separated in momen-tum space and behave like magnetic dipoles [13,24,25]. Arecent player on the scene is a type-II Weyl semimetal, which
Published by the American Physical Society under the terms of theCreative Commons Attribution 4.0 International license. Furtherdistribution of this work must maintain attribution to the author(s)and the published article’s title, journal citation, and DOI.
does not conserve Lorentz invariance in that its Weyl conesare tilted and the electron- and hole-like pockets intersect atthe Fermi surface [26]. Open Fermi surfaces, anisotropic chi-ralities, and unconventional anomalous Hall effect are amongthe unusual features of type-II Weyl semimetals. Type-II Weylfermions are often associated with gigantic magnetoresistance[24,25]. ARPES studies along with parallel first-principlescalculations on MoTe2, WTe2, MoP2, and WP2 [27–30] con-firm their type-II Weyl characteristics. These advances havespurred the exploration of type-II Weyl states in other binarycompounds of Mo and W. Transition metal diarsenides havedrawn special attention due to their high magnetoresistanceand carrier density-of-states [31].
Recent reports of topological properties and the origin ofhigh magnetoresistance in MoAs2 present contradictory re-sults [32–34]. A first-principles calculation finds states withnontrivial Z2 index and suggests high magnetoresistance toresult from electron-hole compensation [32]. However, an-other study reports trivial band structures and argues thatthe high magnetoresistance results from carrier motion onthe Fermi surface, which is enriched via the open-orbittopology [33]. A quantum oscillation experiment comple-mented by first-principles calculations indicates the existenceof open-orbits in MoAs2 [34]. The need for a comprehensiveexperimental and theoretical analysis of the electronic struc-ture of MoAs2 and its sister compound WAs2 is thus clear.A new level of understanding of the electronic structures canalso be expected through the delineation of the terminationdependence of the electronic structure that has not yet beenreported. To date, ARPES measurements have also not been
2643-1564/2021/3(2)/023170(11) 023170-1 Published by the American Physical Society
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
FIG. 1. Crystal structure, electronic transport, and bulk band structure of MoAs2. (a) Conventional unit cell of MoAs2. Purple and greenspheres refer to Mo and As atoms, respectively. (b) Conventional 3D Brillouin zone of MoAs2 with high-symmetry points labeled. Orangeand green lines represent the conventional (001) and (100) surface projection, respectively. (c) Transverse magnetoresistance isotherms takenat different temperatures. (d) Resistivity measured as a function of temperature in zero field (dark red colored symbols) and in a field of 9T applied perpendicular to current (orange-colored symbols). (e) Bulk band structure of MoAs2 without SOC. Linearly crossed bands areenclosed in the red rectangles. (f) Bulk band structure of MoAs2 with SOC.
reported on the related compound WAs2, which belongs to thesame crystal group as MoAs2 but with a stronger spin-orbitcoupling (SOC) strength.
Here we report a systematic ARPES study of TAs2
(T = Mo, W) with parallel theoretical calculations. Electronicstructure of MoAs2 is delineated in two different cleavageplanes. Both surfaces demonstrate the existence of trivial sur-face states. Importantly, the Dirac-like dispersions seen on the(001) surface are formed by trivial bands. We also reveal thepresence of high magnetoresistance and similar Fermi surfacefeatures on the (001) surface of WAs2. Since MoAs2 andWAs2 both exhibit metallic band structures at low tempera-tures with highly populated trivial metallic surface states, ourstudy indicates that topological semimetallic states are not thekey for generating high magnetoresistance in these materials.
II. METHODS
A. Sample growth and characterization
The single crystals of MoAs2 and WAs2 were grown usingthe chemical vapor transport method with iodine as transport-ing agent [35]. The crystals formed needlelike structures withdimensions ∼ 1 × 0.8 × 0.4 mm3. The chemical compositionwas proven by energy-dispersive x-ray analysis using an FEIscanning-electron microscope equipped with an EDAX Gen-esis XM4 spectrometer. The crystal structure was examined atroom temperature on a Kuma-Diffraction KM4 four-circle x-
ray diffractometer equipped with a CCD camera using Mo Kα
radiation. The experiment confirmed the monoclinic crystalstructure and the lattice constants in accord with the previ-ously reported values [35]. Electrical resistivity measurementswere performed over 2 to 300 K employing a conventionalfour-point ac technique implemented in a Quantum DesignPPMS platform. Electrical contacts were made using silverepoxy paste. A perpendicular magnetic field was applied tomeasure the transverse magnetoresistance.
B. Spectroscopic surface measurements
Synchrotron-based ARPES measurements were performedat the Advanced Light Source (ALS), Berkeley, at beamlines4.0.3, 7.0.2, and 10.0.1 equipped with high-efficiency R8000and R4000 electron analyzers. The energy resolution was setto be better than 20 meV. The angular resolution was set to bebetter than 0.2◦ for all measurements. Samples were cleavedin situ and measured at 15 to 25 K in a vacuum better than10−10 Torr. They were found to be very stable and withoutdegradation for the typical measurement period of 20 hours.LEED measurements for structural analysis were performedat the ALS beamline 4.0.3 at a base pressure of better than10−10 Torr in the preparation chamber. Samples were cleavedin the main chamber at a temperature of 80 K and movedto the preparation chamber for room-temperature LEED. Thesample was further characterized by Laue diffraction.
023170-2
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
FIG. 2. Electronic structure of MoAs2 in the (001) plane. (a) Experimental Fermi surface map where high-symmetry points of the Brillouinzone are marked. Red lines represent the constructed Brillouin zone. The map was obtained using photon energy of 90 eV. (b) Calculated Fermimap. (c) Dispersion measurements along the Y -�-Y direction obtained at a photon energy of 98 eV. (d) Second-derivative plot of dispersionmap in (c). (e) Calculated dispersion map along the Y -�-Y direction. All data were collected at the ALS beamline 4.0.3 at a temperatureof 20 K. The orange dotted curves are guides to the eye to compare theory and experimental plots. The blue color represents the bulk bandwhereas the red color denotes the surface band in the calculations.
FIG. 3. Electronic structure of MoAs2 (100) surface. (a) Measured Fermi surface map of the MoAs2 (100) plane. Dashed black linesrepresent the constructed Brillouin zone. (b) Calculated Fermi surface map. (c) Electronic band dispersion along the Y -�-Y direction.(d) Calculated dispersion map along the Y -�-Y direction. (e) Electronic band dispersion along the M-Z-M direction. Data were collectedat the ALS beamline 10.0.1 at a temperature of 15 K using 70 eV photon energy. The orange dotted curves serve as guides to the eye tocompare theory and experimental plots. Blue color denotes surface state and red color represent the bulk state in the calculations.
023170-3
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
FIG. 4. Transport properties and the electronic structure of WAs2 of the (001) plane. (a) Resistivity as a function of temperature measuredin zero field (dark red curve) and in a transverse field of 9 T (orange curve). (b) Transverse magnetoresistance isotherms measured as afunction of the field at different temperatures. (c) Bulk band structure of WAs2 without SOC. (d) Bulk band structure of WAs2 with SOC. (e)Measured Fermi surface map of WAs2 at the photon energy of 35 eV. (f) Energy-momentum dispersion of WAs2 along the Y1-X -Y1 direction.(g) Energy-momentum dispersion of WAs2 along the Y -�-Y direction. All data were collected at the ALS beamline 7.0.2 at a temperature of20 K.
C. First-principles calculations
Electronic structure was calculated by using the Vi-enna ab initio simulation package (VASP) [36] based onthe density-functional theory (DFT) [37] with the projec-tor augmented wave (PAW) method [36,38]. We used thegeneralized-gradient approximation (GGA) [39] to modelexchange-correlation effects. The energy cutoff of the planewave basis set was 400 eV, and the size of the k mesh was16 × 16 × 7. An effective tight-binding model Hamiltonianwas obtained by projecting first-principles results onto Wan-nier orbitals using the VASP2WANNIER90 [40]. The Mo dand As p orbitals were included to generate Wannier func-
tions. We calculated the surface states by using an iterativeGreen’s function method with the WannierTools package [41].
III. RESULTS AND ANALYSIS
A. Crystal structure and sample characterization
MoAs2 crystallizes in a monoclinic structure in the C2/msymmetry group (#12) with lattice parameters: a = 9.064(7)Å, b = 3.987(1) Å, c =7.7182(9) Å, and β= 119.37(1)◦[31,35], see Fig. 1(a). The conventional bulk Brillouin zoneand its 2D projections onto the (100) and (001) surfacesare shown in Fig. 1(b). The temperature dependence of the
023170-4
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
FIG. 5. Experimental geometry for ARPES measurements.
electrical resistivity of MoAs2 is presented in Fig. 1(d). At300 K, the resistivity is about 190 μ� cm and decreasesdown to 2.6 μ� cm at 2 K. The large residual resistivityratio (RRR = ρ300K/ρ2K ) of 79 verifies high quality of thecrystal measured. As seen in Fig. 1(d), magnetic field of 9 Tapplied perpendicular to electric current hardly alters ρ(T ).The transverse magnetoresistance (MR) taken as a function ofthe field at various temperatures from the range 2-200 K ispresented in Fig. 1(c). At low temperatures, the magnitude ofMR is enhanced (MR = 107% at T = 2 K and μ0H = 9 T),and thus signals the possibility of MoAs2 hosting topologicalstates and/or harboring electron-hole compensation. More-over, the observed deviation of MR from the Kohler’s rule canbe associated with the behavior in a multiband system withvariable carrier densities [31]. Bulk band structure of MoAs2
without and with the inclusion of spin-orbit coupling effectsis presented in Figs. 1(e) and 1(f), respectively. The bands inthe vicinity of the Fermi level give an impression of the Diracdispersion in the regions enclosed in red rectangles (0.8 eVabove the Fermi level near L and 1 eV below the Fermi levelnear the Z point). These Dirac-like crossings are seen to take
FIG. 7. Bulk-band structure of MoAs2 with spin-orbit coupling.Topological invariants were calculated by artificially shifting theFermi level (dashed red line) to lie between bands 2 and 3.
place away from the high-symmetry points. Note that theseDirac-like crossings are not robust against spin-orbit couplingas gaps are opened up when spin-orbit coupling effects areincluded in the computations. Our Z2 calculations on MoAs2
show that it is topologically trivial with Z2= (0;000) when theFermi level lies between the bands 2 and 3. It can, however,support a weak topological state with Z2 = (0;111) if theFermi level is artificially placed to lie between bands 1 and2, see Appendix C for details.
B. Observation of trivial band structures on the (001) plane
We carried out ARPES measurements using a VUV photonsource which allows surface-sensitive measurements. Elec-tronic structures of the MoAs2 (001) surface are presentedin Fig. 2. The experimental Fermi surface in Fig. 2(a) con-sists of multiple Fermi pockets indicating the metallic natureof MoAs2. A bridge-like pair of lines at the � point is re-lated to the surface bands. The experimental Fermi surfaceis reasonably captured by our first-principles calculations[Fig. 2(b)], some discrepancies can be attributed to matrix-elements effects [42,43]. We draw orange-colored overlayplot to directly compare theory and experiment. Figure 2(c)displays the dispersion along the Y -�-Y direction. The innerlinear band marked by α, which disperses linearly does notchange shape and size with photon energy, and manifests a
FIG. 6. LEED and Laue measurements. (a) LEED pattern of cleaved surface 1. (b) LEED pattern of cleaved surface 2. (c) Laue diffractionpattern of natural flat surface.
023170-5
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
FIG. 8. Photon-energy dependent electronic dispersions and their second derivative plots along the Y -�-Y direction on the (001) surfacein MoAs2. (a) Dispersion maps along the Y -�-Y direction for different photon energies as noted on the plots. (b) Second derivative plotscorresponding to the maps presented in panel (a). All data were collected at the ALS beamline 4.0.3. at a temperature of 20 K.
surface-originated Dirac-like dispersion. The α-band is seensurrounded by the electron-like band marked β, which be-comes stronger with varying photon energy, indicating itsbulk nature. In particular, we do not see the presence of thisbulk band in the Fermi surface map measured at a photonenergy of 90 eV. Figure 2(d) shows a second-derivative plotof the map of Fig. 2(c) which highlights the linear crossingsof the bands. In Fig. 2(e), the calculated dispersion map ispresented. It reasonably captures the main bands observed inthe experiment. Our theoretical calculations support our view
that the α is a surface band and β is a bulk band. Lower part ofthe α bands are not seen as they are buried in the bulk bands.
C. Electronic structure of the (100) plane
We now consider the surface-dependent electronic struc-ture of MoAs2. Figure 3(a) shows that the Fermi surface mapfor the (100) plane is distinctly different from that for the(001) plane discussed in the preceding section. Approximatelycircular pockets are separated by a pair of lines. Extended
FIG. 9. ARPES measured (a) Dispersion map, (b) MDCs, and (c) EDCs along the Y -�-Y direction on the (001) surface. The data weretaken at 20 K with photon energy of 92 eV. The dotted lines on the MDCs are guides to the eye.
023170-6
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
Fermi map here consists of multiple Brillouin zones presentsa dumbbell shape. The rod-like feature along the �-Z di-rection corresponds to electron-like bands. The calculatedFermi surface is presented in Fig. 3(b) and reasonably matchesthe experimental Fermi surface. Our data does not resolveall the features seen in the theoretical plot due presumablyto the effects of experimental resolution and the ARPESmatrix element. Figure 3(c) shows the dispersion along theY -�-Y where multiple bands can be seen in the vicinity of� that cross the Fermi level. In Fig. 3(d), the first-principlescalculations along the �-Y direction demonstrate the surfacestates, which however are topologically trivial. Similarly, inFig. 3(e), a pair of electron pockets can be seen in the vicinityof the Z point. A hole-like band appears at a higher bindingenergy and does not touch the electron pocket, an obviousgap can be seen. Interestingly, the gapless Dirac-like statesare not seen in Figs. 3(c) and 3(e) (see Appendix D fordetails).
D. Electronic structure of WAs2
WAs2 allows us to gain insight into the effects of tun-ing the strength of spin-orbit coupling in the transition-metaldiarsenides by substituting Mo with W. Figure 4 shows thetransport behavior and the detailed electronic band structuresfor the (001) surface of WAs2. The behavior of zero-field ρ(T )
and transverse MR is rather similar to that in MoAs2 [see Fig.4(a) and 4(b)]. However, RRR of WAs2 is as large as 200(ρ300 K = 140 μ�cm, ρ2 K = 0.7 μ�cm), and MR measuredat T = 2 K and μ0H = 9 T reaches nearly 1200%. As canbe inferred from Fig. 4(a), in a transverse field of 9 T, theresistance increases with decreasing temperature below about40 K, and then forms a plateau, characteristic of semimetalswith similar concentrations of different charge carriers. Thebulk bands in WAs2 are presented in Figs. 4(c) and 4(d). Fig-ure 4(c) shows bulk band without spin-orbit coupling. It doesnot indicate the presence of gapless Dirac-like dispersion. Theinclusion of spin-orbit coupling [Fig. 4(d)] widens the gapbetween the linearly dispersing bands; our calculations areconsistent with a previous study [32]. The Fermi surface ofWAs2 contains multiple Fermi pockets suggesting a metallicnature of the material. The Fermi surface shows a dumbbell-shaped feature with the middle of its handle located at the �
point. In order to examine the Dirac state in WAs2, the disper-sion maps were taken along the high-symmetry directions asshown in Figs. 4(f) and 4(g). Figure 4(f) shows the dispersionalong the Y1-X -Y1 direction as consisting of hole-like bands.The dispersion along the Y -�-Y direction also shows trivialbands with the band structure dominated by the bulk bands.In contrast to MoAs2, WAs2 does not possess a surface Dirac-like dispersion in this direction.
FIG. 10. Photon-energy-dependent electronic band dispersions along the M-Z-M direction from the (100) surface of MoAs2. (a) Experi-mental spectra at various indicated photon energies. (b) Second derivative plots corresponding to the spectra of panel (a). All the data werecollected at the ALS beamline 10.0.1 at 15 K.
023170-7
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
IV. CONCLUSIONS
We have carried out a systematic ARPES study oftransition-metal diarsenides TAs2 (T = Mo, W) in con-junction with first-principles calculations. Surface electronicstructures for the (001) and (100) surfaces are found to bequite different with both surfaces exhibiting the presence ofmultiple metallic Fermi surface pockets. Our symmetry anal-ysis of the bulk band structures shows clearly that neitherof these diarsenides supports a topological insulator state.This, along with the fact that these compounds respect timereversal as well as inversion symmetry, would seem to ruleout their being either an intrinsic Dirac or a Weyl semimetaleven though the band structures display some Dirac-likelinearly-dispersing features. Our study highlights the impor-tance of identifying the cleavage plane in electronic structurestudies of low-symmetry systems.
ACKNOWLEDGMENTS
M.N. is supported by the Air Force Office of Scientific Re-search under Award No. FA9550-17-1-0415 and the NationalScience Foundation (NSF) CAREER Award No. DMR-1847962. The work at Northeastern University was supportedby the U.S. Department of Energy (DOE), Office of Science,Basic Energy Sciences Grant No. DE-FG02-07ER46352, andbenefited from Northeastern University’s Advanced ScientificComputation Center (ASCC) and the NERSC supercomput-
ing center through DOE Grant No. DE-AC02-05CH11231.H.L. acknowledges the support by the Ministry of Scienceand Technology (MOST) in Taiwan under Grant No. MOST109-2112-M-001-014-MY3. The work at TIFR Mumbai wassupported by the Department of Atomic Energy of the Gov-ernment of India under Project No. 12-R&D-TFR-5.10-0100.This research used resources of the Advanced Light Source,a U.S. Department of Energy Office of Science User Facility,under Contract No. DE-AC02-05CH11231. We thank Sung-Kwan Mo, Eli Rotenberg, Aaron Bostwick, and Chris Jozwiakfor beamline assistance at the LBNL.
APPENDIX A: EXPERIMENTAL GEOMETRYOF THE ARPES MEASUREMENTS
The photoemission intensity (I0) obtained in ARPES mea-surements is directly proportional to matrix element Mk
f ,i|2which, in turn, is proportional to |〈φk
f |||�ε.�x|||φki 〉|2, where φk
i
and φkf are the initial and final state wave functions of pho-
toelectrons, respectively [44]. �ε and �x denote the unit vectorgiving the direction of the electric field of the incoming photonand the unit position vector of electrons, respectively.
We present our experimental ARPES geometry in Fig. 5showing that the incoming photon beam consists of a mixtureof s and p polarization. Both the analyzer slit and the incomingphotons lie in the mirror plane defined by the analyzer slit and
FIG. 11. Experimentally measured dispersion map, MDCs, and EDCs along the (a) M-Z-M and (b) Y -�-Y direction on the (100) surfaceof MoAs2. Data were collected at the ALS beamline 10.0.1 at 15 K.
023170-8
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
FIG. 12. Experimental Fermi surface map of WAs2 (a) from the(001) surface of WAs2 and (b) the corresponding second-derivativeplot of the Fermi surface. The data were collected at the ALS beam-line 7.0.2 at 20 K using 35 eV photons.
the sample surface normal. In this setup �ε.�x must be either oddor even to give a nonzero photo-intensity [32,45].
APPENDIX B: LEED MEASUREMENTS OF CLEAVEDSURFACE OF MoAs2
In order to study the cleaved surface, we performed LEEDand Laue spectroscopy measurements which are summarizedin Fig. 6. Figures 6(a) and 6(b) show two different representa-tive cleaving planes among multiple possible cleaving planes,LEED measurements demonstrate that MoAs2 does not havea preferred cleaving plane. Many samples were cleaved to in-spect the preferred cleaving plane in MoAs2 which concludedaforementioned results. Laue diffraction pattern of naturalflat surface is presented in Fig. 6(c). The lack of preferredcleaving plane in monoclonic transition metal diarsenides canbe attributed to low crystal symmetry and absence of van derWaals interaction.
APPENDIX C: ELECTRONIC STRUCTURESON THE (001) SURFACE OF MoAs2
Figure 7 presents the bulk-band structure of MoAs2.The Fermi energy was artificially placed to lie between thebands 2 and 3. Our Z2 calculations for this band structureyield a trivial band structure. Figure 8 shows experimentalphoton-energy-dependent ARPES spectra for MoAs2 alongthe Y -�-Y direction and their second derivative plots. Thesedata exhibit the presence of a gapless Dirac-like dispersion onthe (001) plane. An electron-like band in the vicinity of the� point close to the Fermi level is suppressed at the photonenergy of 92 eV. However α-band [see Fig. 2(c)] does notdisperse with photon energies indicating the surface state (seeFig. 8). In Fig. 9, we present MDCS and EDCs of dispersionmap along the Y -�-Y direction which find the presence ofgapless Dirac-like dispersion.
APPENDIX D: ELECTRONIC STRUCTURES ON THE (100)SURFACE OF WAs2
Figure 10 presents the photon-energy-dependent disper-sion maps along the M-Z-M direction and correspondingsecond derivative plots. The dispersion maps at different pho-ton energies demonstrate the absence of gapless Dirac-likestate along this direction. MDCs and EDCs plots of dispersionmaps along the M-Z-M and M-�-M (see Fig. 11) further con-firm the absence of gapless Dirac-like state on the (100) plane.
APPENDIX E: ELECTRONIC STRUCTUREOF THE (001) SURFACE OF WAs2.
Figures 12 to 14 present electronic structures of WAs2.The Fermi surface is seen to be quite different from that ofMoAs2. Photon-energy-dependent spectra along the Y -�-Ydirection (see Fig. 13) indicate the presence of non-dispersivebands at the � point near the Fermi level. MDCs and EDCsalong Y -�-Y and Y1-X -Y1 are presented in Fig. 14 provide aclear indication of lack of Dirac states. The dispersion mapsof WAs2 are quite different from those of MoAs2.
FIG. 13. Photon-energy-dependent spectral maps along the Y -�-Y direction on the (001) surface of WAs2. Data were collected at the ALSbeamline 7.0.2. at 20 K.
023170-9
GYANENDRA DHAKAL et al. PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
FIG. 14. Dispersion map, MDCs and EDCs along the (a) Y -�-Y direction, and the (b) Y1-X -Y1 direction. Data were collected at the ALSbeamline 7.0.2 at 20 K using 35 eV photons.
[1] M. Z. Hasan and C. L. Kane, Colloquium: Topological insula-tors, Rev. Mod. Phys. 82, 3045 (2010).
[2] J. E. Moore, The birth of topological insulators, Nature(London) 464, 194 (2010).
[3] X.-L. Qi, and S.-C. Zhang, Topological insulators and super-conductors, Rev. Mod. Phys. 83, 1057 (2011).
[4] M. Z. Hasan, S.-Y. Xu, and M. Neupane, Topological In-sulators, topological Dirac semimetals, topological crystallineinsulators, and topological Kondo knsulators. in Topological In-sulators: Fundamentals and Perspectives, edited by F. Ortmann,S. Roche, and S. O. Valenzuela (John Wiley & Sons, New York,2015).
[5] A. Bansil, H. Lin, and T. Das, Colloquium: Topological bandtheory, Rev. Mod. Phys. 88, 021004 (2016).
[6] S. Murakami, Phase transition between the quantum spin Halland insulator phases in 3D: Emergence of a topological gaplessphase, New J. Phys. 9, 356 (2007).
[7] S. M. Young, S. Zaheer, J. C. Y. Teo, C. L. Kane, E. J. Mele,and A. M. Rappe, Dirac Semimetal in Three Dimensions, Phys.Rev. Lett. 108, 140405 (2012).
[8] Z. Wang, H. Weng, Q. Wu, X. Dai, and Z. Fang, Three-dimensional Dirac semimetal and quantum transport in Cd3As2,Phys. Rev. B 88, 125427 (2013).
[9] M. Neupane, S.-Y. Xu, R. Sankar, N. Alidoust, G. Bian, C. Liu,I. Belopolski, T.-R. Chang, H.-T. Jeng, H. Lin, A. Bansil, F.Chou, and M. Z. Hasan, Observation of a three-dimensional
topological Dirac semimetal phase in high-mobility Cd3As2,Nat. Commun. 5, 3786 (2014).
[10] B.-J. Yang and N. Nagaosa, Classification of stable three-dimensional Dirac semimetals with nontrivial topology,Nat. Commun. 5, 4898 (2014).
[11] M. Neupane, N. Alidoust, M. M. Hosen, J.-X. Zhu, K. Dimitri,S.-Y. Xu, N. Dhakal, R. Sankar, I. Belopolski, D. S. Sanchez,T.-R. Chang, H.-T. Jeng, K. Miyamoto, T. Okuda, H. Lin, A.Bansil, D. Kaczorowski, F. C. Chou, M. Z. Hasan, and T.Durakiewicz, Observation of the spin-polarized surface state ina noncentrosymmetric superconductor BiPd, Nat. Commun. 7,13315 (2016).
[12] S. M. Young and C. L. Kane, Dirac Semimetals in Two Dimen-sions, Phys. Rev. Lett. 115, 126803 (2015).
[13] X. Wan, A. M. Turner, A. Vishwanath, and S. Savrasov, Topo-logical semimetal and Fermi-arc surface states in the electronicstructure of pyrochlore iridates, Phys. Rev. B 83, 205101(2011).
[14] S.-M. Huang, S.-Y. Xu, I. Belopolski, C.-C. Lee, G. Chang, B.Wang, N. Alidoust, G. Bian, M. Neupane, C. Zhang, S. Jia, A.Bansil, H. Lin, and M. Z. Hasan, A Weyl Fermion semimetalwith surface Fermi arcs in the transition metal monopnictideTaAs class, Nat. Commun. 6, 7373 (2015).
[15] H. Weng, C. Fang, Z. Fang, B. A. Bernevig, and X. Dai,Weyl Semimetal Phase in Noncentrosymmetric Transition-Metal Monophosphides, Phys. Rev. X 5, 011029 (2015).
023170-10
CLEAVING PLANE-DEPENDENT ELECTRONIC … PHYSICAL REVIEW RESEARCH 3, 023170 (2021)
[16] S.-Y. Xu, I. Belopolski, N. Alidoust, M. Neupane, G. Bian, C.Zhang, R. Sankar, G. Chang, Z. Yuan, C.-C. Lee, S.-M. Huang,H. Zheng, J. Ma, D. S. Sanchez, B. Wang, A. Bansil, F. Chou,P. P. Shibayev, H. Lin, S. Jia et al., Discovery of a Weyl fermionsemimetal and topological Fermi arcs, Science 349, 613(2015).
[17] B. Q. Lv, H. M. Weng, B. B. Fu, X. P. Wang, H. Miao, J. Ma,P. Richard, X. C. Huang, L. X. Zhao, G. F. Chen, Z. Fang, X.Dai, T. Qian, and H. Ding, Experimental Discovery of WeylSemimetal TaAs, Phys. Rev. X 5, 031013 (2015).
[18] I. Belopolski, S.-Y. Xu, D. S. Sanchez, G. Chang, C. Guo,M. Neupane, H. Zheng, C.-C. Lee, S.-M. Huang, G. Bian, N.Alidoust, T.-R. Chang, B. K. Wang, X. Zhang, A. Bansil, H.-T.Jeng, H. Lin, S. Jia, and M. Z. Hasan, Criteria for DirectlyDetecting Topological Fermi Arcs in Weyl Semimetals, Phys.Rev. Lett. 116, 066802 (2016).
[19] M. Z. Hasan, S.-Y. Xu, and G. Bian, Topological insulators,topological superconductors and Weyl fermion semimetals: dis-coveries, perspectives and outlooks, Phys. Scr. T164, 014001(2015).
[20] G. Bian, T.-R. Chang, R. Sankar, S.-Y. Xu, H. Zheng, T.Neupert, C.-K. Chiu, S.-M. Huang, G. Chang, I. Belopolski,D. S. Sanchez, M. Neupane, N. Alidoust, C. Liu, B. K. Wang,C.-C. Lee, H.-T. Jeng, C. Zhang, Z. Yuan, S. Jia et al. Topo-logical nodal-line fermions in spin-orbit metal PbTaSe2, Nat.Commun. 7, 10556 (2016).
[21] M. Neupane, I. Belopolski, M. M. Hosen, D. S. Sanchez, R.Sankar, M. Szlawska, S.-Y. Xu, K. Dimitri, N. Dhakal, P.Maldonado, P. M. Oppeneer, D. Kaczorowski, F. C. Chou, M. Z.Hasan, and T. Durakiewicz, Observation of topological nodalfermion semimetal phase in ZrSiS, Phys. Rev. B 93, 201104(R)(2016).
[22] M. M. Hosen, K. Dimitri, I. Belopolski, P. Maldonado, R.Sankar, N. Dhakal, G. Dhakal, T. Cole, P. M. Oppeneer, D.Kaczorowski, F. Chou, M. Z. Hasan, T. Durakiewicz, and M.Neupane, Tunability of the topological nodal-line semimetalphase in ZrSi X -type materials (X = S, Se, Te), Phys. Rev. B95, 161101(R) (2017).
[23] C. Sims, M. M. Hosen, H. Aramberri, C.-Y. Huang, G. Dhakal,K. Dimitri, F. Kabir, S. Regmi, X. Zhou, T.-R. Chang, H. Lin,D. Kaczorowski, N. Kioussis, and M. Neupane, Termination-dependent topological surface states in nodal-loop semimetalHfP2, Phys. Rev. Materials 4, 054201 (2020).
[24] M. Z. Hasan, S.-Y. Xu, I. Belopolski, and S.- M. Huang, Dis-covery of Weyl Fermion Semimetals and Topological Fermi ArcStates, Annu. Rev. Condens. Matter Phys. 8, 289 (2017).
[25] N. P. Armitage, E. J. Mele, and A. Vishwanath, Weyl and Diracsemimetals in three-dimensional solids, Rev. Mod. Phys. 90,015001 (2018).
[26] A. A. Soluyanov, D. Gresch, Z. Wang, Q. Wu, M. Troyer, X.Dai, and B. A. Bernevig, Type-II Weyl semimetals, Predictionof Weyl semimetal in orthorhombic MoTe2, Nature (London)527, 495 (2015).
[27] Y. Sun, S.-C. Wu, M. N. Ali, C. Felser, and B. Yan, Spectro-scopic evidence for a type II Weyl semimetallic state in MoTe2,Phys. Rev. B 92, 161107(R) (2015).
[28] L. Huang, T. M. McCormick, M. Ochi, Z. Zhao, M.-t. Suzuki,R. Arita, Y. Wu, D. Mou, H. Cao, J. Yan, N. Tridevi, andA. Kaminski, Spectroscopic evidence for a type II Weylsemimetallic state in MoTe2, Nat. Mater. 15, 1155 (2016).
[29] Y. Wu, D. X. Mou, N. H. Jo, K. W. Sun, L. Huang, S. L. Budko,P. C. Canfield, and A. Kaminski, Observation of Fermi arcs inthe type-II Weyl semimetal candidate WTe2, Phys. Rev. B 94,121113(R) (2016).
[30] G. Autès, D. Gresch, M. Troyer, A. A. Soluyanov, and O. V.Yazyev, Robust Type-II Weyl Semimetal Phase in TransitionMetal Diphosphides XP2 (X = Mo, W), Phys. Rev. Lett. 117,066402 (2016).
[31] J. Wang, L. Li, W. You, T. Wang, C. Cao, J. Dai and Y. Li,Magnetoresistance and robust resistivity plateau in MoAs2, Sci.Rep. 7, 15669 (2017).
[32] J. Chen, Y.-K. Li, J. Dai, and C. Cao, Electronic structure andtopological properties of centrosymmetric MoAs2/WAs2 fromfirst principles, Sci. Rep. 7, 10491 (2017).
[33] R. Lou, Y. F. Xu, L.-X. Zhao, Z.-Q. Han, P.-J. Guo, M. Li,J.-C. Wang, B.-B. Fu, Z.-H. Liu, Y.-B. Huang, P. Richard, T.Qian, K. Liu, G.-F. Chen, H. M. Weng, H. Ding, and S.-C.Wang, Observation of open-orbit Fermi surface topology inthe extremely large magnetoresistance semimetal MoAs2, Phys.Rev. B 96, 241106(R) (2017).
[34] R. Singha, A. Pariari, G. K. Gupta, T. Das, and P. Mandal,Probing the Fermi surface and magnetotransport properties ofMoAs2, Phys. Rev. B 97, 155120 (2018).
[35] J. J. Murray, J. B. Taylor, and L. Usner, Halogen transportof molybdenum arsenides and other transition metal pnictides,J. Cryst. Growth 15, 231 (1972).
[36] G. Kresse and D. Joubert, From ultrasoft pseudopotentials tothe projector augmented-wave method, Phys. Rev. B 59, 1758(1999).
[37] P. Hohenberg and W. Kohn, Inhomogeneous electron gas, Phys.Rev. 136, B864 (1964).
[38] G. Kresse and J. Furthmuller, Efficient iterative schemes forab initio total-energy calculations using a plane-wave basis set,Phys. Rev. B 54, 11169 (1996).
[39] J. P. Perdew, K. Burke, and M. Ernzerhof, Generalized Gra-dient Approximation Made Simple, Phys. Rev. Lett. 77, 3865(1996).
[40] N. Marzari and D. Vanderbilt, Maximally localized generalizedWannier functions for composite energy bands, Phys. Rev. B56, 12847 (1997).
[41] Q. Wu, S. Zhang, H.-F. Song, M. Troyer, and A. A. Soluyanov,WannierTools: An open-source software package for noveltopological materials, Comput. Phys. Commun. 224, 405(2018).
[42] A. Bansil and M. Lindroos, Importance of Matrix Elementsin the ARPES Spectra of BISCO, Phys. Rev. Lett. 83, 5154(1999).
[43] M. R. Scholz, J. Sanchez-Barriga, J. Braun, D. Marchenko, A.Varykhalov, M. Lindroos, Y. J. Wang, H. Lin, A. Bansil, J. Minr,H. Ebert, A. Volykhov, L. V. Yashina, and O. Rader, Reversal ofthe Circular Dichroism in Angle-Resolved Photoemission fromBi2Te3, Phys. Rev. Lett. 110, 216801 (2013).
[44] A. Damascelli, Z. Hussain, and Z.-X. Shen, Angle-resolvedphotoemission studies of the cuprate superconductors, Rev.Mod. Phys. 75, 473 (2003).
[45] S. Tang, C. Zhang, D. Wong, Z. Pedramrazi, H.-Z. Tsai, C. Jia,B. Moritz, M. Claassen, H. Ryu, S. Kahn, J. Jiang, H. Yan, M.Hashimoto, D. Lu, R. G. Moore, C.-C. Hwang, C. Hwang, Z.Hussain, Y. Chen, M. M. Ugeda et al., Quantum spin Hall statein monolayer 1T’-WTe2, Nat. Phys. 13, 683 (2017).
023170-11